CELEX: 32006L0002
Language: en
Date: 2006-01-06 00:00:00
Title: Commission Directive 2006/2/EC of  6 January 2006  amending, for the purposes of its adaptation to technical progress, Annexe II to Directive 96/73/EC of the European Parliament and of the Council on certain methods for quantitative analysis of binary textile fibre mixtures   (Text with EEA relevance)

10.1.2006   
            
            
               EN
            
            
               Official Journal of the European Union
            
            
               L 5/10
            
         
      COMMISSION DIRECTIVE 2006/2/EC
   of 6 January 2006
   amending, for the purposes of its adaptation to technical progress, Annexe II to Directive 96/73/EC of the European Parliament and of the Council on certain methods for quantitative analysis of binary textile fibre mixtures
   (Text with EEA relevance)
   THE COMMISSION OF THE EUROPEAN COMMUNITIES,
   Having regard to the Treaty establishing the European Community,
   Having regard to Directive 96/73/EC of the European Parliament and of the Council of 16 December 1996 on certain methods for quantitative analysis of binary textile fibre mixtures (1), and in particular Article 5(2) thereof,
   Whereas:
   
               (1)
            
            
               Directive 96/74/EC of the European Parliament and the Council of 16 December 1996 on textile names (2) requires labelling to indicate the fibre composition of textile products, with checks being carried out by analysis on the conformity of these products with indications given on the label.
            
         
               (2)
            
            
               Uniform methods for quantitative analysis of binary textile fibre mixtures are provided in Directive 96/73/EC.
            
         
               (3)
            
            
               On the basis of recent findings by a technical working group, Directive 96/74/EC was adapted to technical progress, by adding the fibres polylactide and elastomultiester to the list of fibres set out in the Annexes I and II to that Directive.
            
         
               (4)
            
            
               It is therefore necessary to define uniform test methods for polylactide and elastomultiester.
            
         
               (5)
            
            
               Directive 96/73/EC should therefore be amended accordingly.
            
         
               (6)
            
            
               The measures provided for in this Directive are in accordance with the opinion of the Committee for Directives relating to Textile Names and Labelling,
            
         HAS ADOPTED THIS DIRECTIVE:
   Article 1
   Annex II to Directive 96/73/EC is amended in accordance with the Annex to this Directive.
   Article 2
   1.   Member States shall bring into force the laws, regulations and administrative provisions necessary to comply with this Directive by 6 January 2007 at the latest. They shall forthwith communicate to the Commission the text of those provisions and a correlation table between those provisions and this Directive.
   When Member States adopt those provisions, they shall contain a reference to this Directive or be accompanied by such a reference on the occasion of their official publication. Member States shall determine how such reference is to be made.
   2.   Member States shall communicate to the Commission the text of the main provisions of national law which they adopt in the field covered by this Directive.
   Article 3
   This Directive shall enter into force on the twentieth day following that of its publication in the Official Journal of the European Union.
   Article 4
   This Directive is addressed to the Members States.
   
      Done at Brussels, 6 January 2006.
      
         
            For the Commission
         
         Günter VERHEUGEN
         
         
            Vice-President
         
      
   
   
      (1)  OJ L 32, 3.2.1997, p. 1. Directive as amended by Regulation (EC) No 1882/2003 (OJ L 284, 31.10.2003, p. 1).
   
      (2)  OJ L 32, 3.2.1997, p. 38. Directive as last amended by Commission Directive 2004/34/EC (OJ L 89, 26.3.2004, p. 35).
   
      ANNEX
      Chapter 2 of Annex II to Directive 96/73/EC is amended as follows (1):
      
                  1.
               
               
                  The special methods — Summary Table is replaced by the following:
                  ‘2.   SPECIAL METHODS — SUMMARY TABLE
                  
                              Methods
                           
                           
                              Field of application
                           
                           
                              Reagent
                           
                        
                              No 1
                           
                           
                              Acetate
                           
                           
                              Certain other fibres
                           
                           
                              Acetone
                           
                        
                              No 2
                           
                           
                              Certain protein fibres
                           
                           
                              Certain other fibres
                           
                           
                              Hypochlorite
                           
                        
                              No 3
                           
                           
                              Viscose, cupro or certain types of modal
                           
                           
                              Cotton
                           
                           
                              Formic acid and zinc chloride
                           
                        
                              No 4
                           
                           
                              Polyamide or nylon
                           
                           
                              Certain other fibres
                           
                           
                              Formic acid, 80 % m/m
                           
                        
                              No 5
                           
                           
                              Acetate
                           
                           
                              Triacetate
                           
                           
                              Benzyl alcohol
                           
                        
                              No 6
                           
                           
                              Triacetate or polylactide
                           
                           
                              Certain other fibres
                           
                           
                              Dichloromethane
                           
                        
                              No 7
                           
                           
                              Certain cellulose fibres
                           
                           
                              Polyester or elastomultiester
                           
                           
                              Sulphuric acid, 75 % m/m
                           
                        
                              No 8
                           
                           
                              Acrylics, certain modacrylics or certain chlorofibres
                           
                           
                              Certain other fibres
                           
                           
                              Dimethylformamide
                           
                        
                              No 9
                           
                           
                              Certain chlorofibres
                           
                           
                              Certain other fibres
                           
                           
                              Carbon disulphide/acetone, 55.5/44.5 v/v
                           
                        
                              No 10
                           
                           
                              Acetate
                           
                           
                              Certain chlorofibres
                           
                           
                              Glacial acetic acid
                           
                        
                              No 11
                           
                           
                              Silk
                           
                           
                              Wool or hair
                           
                           
                              Sulphuric acid, 75 % m/m
                           
                        
                              No 12
                           
                           
                              Jute
                           
                           
                              Certain animal fibres
                           
                           
                              Nitrogen content method
                           
                        
                              No 13
                           
                           
                              Polypropylene
                           
                           
                              Certain other fibres
                           
                           
                              Xylene
                           
                        
                              No 14
                           
                           
                              Certain other fibres
                           
                           
                              Chlorofibres (homopolymers of vinyl chloride)
                           
                           
                              Concentrated sulphuric acid method
                           
                        
                              No 15
                           
                           
                              Chlorofibres, certain modacrylics, certain elastanes, acetates, triacetates
                           
                           
                              Certain other fibres
                           
                           
                              Cyclohexanone’
                           
                        
            
                  2.
               
               
                  Point 1.2 of method No 1 is replaced by the following:
                  
                              ‘2.
                           
                           
                              wool (1), animal hair (2 and 3), silk (4), cotton (5), flax (7) true hemp (8), jute (9), abaca (10), alfa (11), coir (12), broom (13), ramie (14), sisal (15), cupro (21), modal (22), protein (23), viscose (25), acrylic (26), polyamide or nylon (30), polyester (34) and elastomultiester (45)’.
                           
                        
            
                  3.
               
               
                  Point 1.2 of method No 2 is replaced by the following:
                  
                              ‘2.
                           
                           
                              cotton (5), cupro (21), viscose (25), acrylic (26), chlorofibres (27), polyamide or nylon (30), polyester (34), polypropylene (36), elastane (42), glass fibre (43) and elastomultiester (45)’.
                           
                        
            
                  4.
               
               
                  Point 1.2 of method No 4 is replaced by the following:
                  
                              ‘2.
                           
                           
                              wool (1), animal hair (2 and 3), cotton (5), cupro (21), modal (22), viscose (25), acrylic (26), chlorofibre (27), polyester (34), polypropylene (36), glass fibre (43) and elastomultiester (45)’.
                           
                        
            
                  5.
               
               
                  Method No 6 is amended as follows:
                  
                              (a)
                           
                           
                              Points 1, 2 of method No 6 are replaced by the following:
                              ‘1.   FIELD OF APPLICATION
                              This method is applicable, after removal of non-fibrous matter, to binary mixtures of:
                              
                                          1.
                                       
                                       
                                          triacetate (24) or polylactide (33a)
                                          with
                                       
                                    
                                          2.
                                       
                                       
                                          wool (1), animal hair (2 and 3), silk (4), cotton (5), cupro (21), modal (22), viscose (25), acrylic (26), polyamide or nylon (30), polyester (34), glass fibre (43) and elastomultiester (45).
                                       
                                    Note
                              Triacetate fibres which have received a finish leading to partial hydrolysis cease to be completely soluble in the reagent. In such cases, the method is not applicable.
                              2.   PRINCIPLE
                              The triacetate or polylactide fibres are dissolved out from a known dry mass of the mixture, with dichloromethane. The residue is collected, washed, dried and weighed; its mass, corrected if necessary, is expressed as a percentage of the dry mass of the mixture. The percentage of dry triacetate or polylactide is found by difference’.
                           
                        
                              (b)
                           
                           
                              Point 5 is replaced by the following:
                              ‘5.   CALCULATION AND EXPRESSION OF RESULTS
                              Calculate the results as described in the general instructions. The value of “d” is 1.00, except in the case of polyester and elastomultiester, for which the value of “d” is 1.01’.
                           
                        
            
                  6.
               
               
                  Point 1.2 of method No 7 is replaced by the following:
                  
                              ‘2.
                           
                           
                              Polyester (34) and elastomultiester (45)’.
                           
                        
            
                  7.
               
               
                  Method No 8 is amended as follows:
                  
                              (a)
                           
                           
                              Point 1.2 is replaced by the following:
                              
                                          ‘2.
                                       
                                       
                                          wool (1), animal hair (2 and 3), silk (4), cotton (5), cupro (21), modal (22), viscose (25), polyamide or nylon (30), polyester (34), and elastomultiester (45)’.
                                       
                                    
                        
                              (b)
                           
                           
                              Point 5 is replaced by the following:
                              ‘5.   CALCULATION AND EXPRESSION OF RESULTS
                              Calculate the results as described in the general instructions. The value of “d” is 1,00 except in the following cases:
                              
                                           
                                       
                                       
                                          wool 1,01
                                       
                                    
                                           
                                       
                                       
                                          cotton 1,01
                                       
                                    
                                           
                                       
                                       
                                          cupro 1,01
                                       
                                    
                                           
                                       
                                       
                                          modal 1,01
                                       
                                    
                                           
                                       
                                       
                                          polyester 1,01
                                       
                                    
                                           
                                       
                                       
                                          elastomultiester 1,01’
                                       
                                    
                        
            
                  8.
               
               
                  Point 1.2 of method No 9 is replaced by the following:
                  
                              ‘2.
                           
                           
                              wool (1), animal hair (2 and 3), silk (4), cotton (5), cupro (21), modal (22), viscose (25), acrylic (26), polyamide or nylon (30), polyester (34), glass fibre (43) and elastomultiester (45)’.
                           
                        
            
                  9.
               
               
                  Points 1.1 and 1.2 of method No 13 are replaced by the following:
                  
                              ‘1.
                           
                           
                              polypropylene fibres (36)
                              with
                           
                        
                              2.
                           
                           
                              wool (1), animal hair (2 and 3), silk (4), cotton (5), acetate (19), cupro (21), modal (22), triacetate (24), viscose (25), acrylic (26), polyamide or nylon (30), polyester (34), glass fibre (43) and elastomultiester (45)’.
                           
                        
            
                  10.
               
               
                  Point 1.2 of method No 14 is replaced by the following:
                  
                              ‘2.
                           
                           
                              cotton (5), acetate (19), cupro (21), modal (22), triacetate (24), viscose (25), certain acrylics (26), certain modacrylics (29), polyamide or nylon (30), polyester (34) and elastomultiester (45)’.
                           
                        
            
         (1)  Fibres Numbering: 1. Polyester (34) previously (31), 2. polypropylene (36) previously (33), 3.elastane (42) previously (39), 4. glass fibre (43) previously (40) see Directive 96/74/EC, as amended by Directive 97/37/EC (OJ L 169, 27.6.1997, p. 74).